 
data_shelx
 
_audit_creation_method            'SHELXL-2018/3'
_shelx_SHELXL_version_number      '2018/3'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Ba0.50 Ce Fe0.50 Na3 O17 Si6 Sr0.50 Zn0.50' 
_chemical_formula_weight          822.72

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0817   0.0704
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.3463   0.8444
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Zn'  'Zn'   0.2839   1.4301
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Sr'  'Sr'  -1.5307   3.2498
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ba'  'Ba'  -0.3244   2.2819
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ce'  'Ce'  -0.2486   2.6331
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       orthorhombic
_space_group_IT_number            54
_space_group_name_H-M_alt         'P c c a'
_space_group_name_Hall            '-P 2a 2ac'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x+1/2, -y, z'
 '-x, y, -z+1/2'
 'x+1/2, -y, -z+1/2'
 '-x, -y, -z'
 'x-1/2, y, -z'
 'x, -y, z-1/2'
 '-x-1/2, y, z-1/2'
 
_cell_length_a                    14.5596(4)
_cell_length_b                    5.22130(10)
_cell_length_c                    19.8270(4)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      1507.25(6)
_cell_formula_units_Z             4
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used   10702
_cell_measurement_theta_min     2.4730
_cell_measurement_theta_max     31.2270
 
_exptl_crystal_description        platy
_exptl_crystal_colour             yellow
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     3.626          
_exptl_crystal_F_000              1544
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max                             0.059
_exptl_crystal_size_mid                             0.024
_exptl_crystal_size_min                             0.013
_exptl_absorpt_coefficient_mu     7.951
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type            gaussian
_exptl_absorpt_correction_T_min                     0.750
_exptl_absorpt_correction_T_max                     0.953
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.63a (Rigaku Oxford Diffraction, 2019)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source 'micro-focus sealed X-ray tube'
_diffrn_source_type 'PhotonJet (Mo) X-ray Source'

_diffrn_radiation_monochromator mirror
_diffrn_measurement_device 'four-circle diffractometer'
_diffrn_measurement_device_type 'XtaLAB Synergy, Dualflex, HyPix'
_diffrn_detector 'Hybrid Pixel Array Detector'
_diffrn_detector_type HyPix
_diffrn_detector_area_resol_mean 10.0000
_diffrn_measurement_method 'ω scans'

_diffrn_reflns_number             29642
_diffrn_reflns_av_unetI/netI      0.0167
_diffrn_reflns_av_R_equivalents   0.0396
_diffrn_reflns_limit_h_min        -20
_diffrn_reflns_limit_h_max        19
_diffrn_reflns_limit_k_min        -7
_diffrn_reflns_limit_k_max        7
_diffrn_reflns_limit_l_min        -27
_diffrn_reflns_limit_l_max        28
_diffrn_reflns_theta_min          2.054
_diffrn_reflns_theta_max          31.455
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.942
_diffrn_measured_fraction_theta_full  1.000
_diffrn_reflns_Laue_measured_fraction_max    0.942
_diffrn_reflns_Laue_measured_fraction_full   1.000
_diffrn_reflns_point_group_measured_fraction_max   0.942
_diffrn_reflns_point_group_measured_fraction_full  1.000
_reflns_number_total              2362
_reflns_number_gt                 1902
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection     'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_cell_refinement     'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_data_reduction      'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_structure_solution     ?
_computing_structure_refinement 'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0355P)²+1.8002P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          2362
_refine_ls_number_parameters      140
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0348
_refine_ls_R_factor_gt            0.0246
_refine_ls_wR_factor_ref          0.0665
_refine_ls_wR_factor_gt           0.0628
_refine_ls_goodness_of_fit_ref    1.072
_refine_ls_restrained_S_all       1.072
_refine_ls_shift/su_max           0.002
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ce1 Ce 0.250000 0.500000 0.31864(2) 0.01166(8) Uani 0.986(2) 2 d S T P . .
Sr1 Sr 0.250000 0.500000 0.52469(2) 0.01285(9) Uani 0.323(5) 2 d S T P . .
Ba1 Ba 0.250000 0.500000 0.52469(2) 0.01285(9) Uani 0.677(5) 2 d S T P . .
Zn1 Zn 0.250000 0.000000 0.67170(2) 0.01307(19) Uani 0.170(17) 2 d S T P . .
Fe1 Fe 0.250000 0.000000 0.67170(2) 0.01307(19) Uani 0.830(17) 2 d S T P . .
Na1 Na 0.000000 0.500000 0.500000 0.0254(6) Uani 0.972(8) 2 d S . P . .
Na2 Na 0.06710(12) 0.5104(2) 0.67249(5) 0.0284(5) Uani 1.053(6) 1 d . . P . .
Si1 Si 0.09574(6) 0.96823(14) 0.56596(4) 0.01257(17) Uani 1 1 d . . . . .
Si2 Si 0.10168(5) 0.95859(14) 0.27464(4) 0.01224(17) Uani 1 1 d . . . . .
Si3 Si 0.11097(5) 0.04721(15) 0.41845(3) 0.01217(16) Uani 1 1 d . . . . .
O1 O 0.00581(13) 0.1639(4) 0.41777(9) 0.0166(4) Uani 1 1 d . . . . .
O2 O 0.16775(13) 0.8119(4) 0.61105(9) 0.0182(4) Uani 1 1 d . . . . .
O3 O 0.11758(13) 0.8681(4) 0.48678(8) 0.0160(4) Uani 1 1 d . . . . .
O4 O 0.09658(15) 0.2701(4) 0.56955(9) 0.0192(4) Uani 1 1 d . . . . .
O5 O 0.000000 0.8590(5) 0.250000 0.0182(6) Uani 1 2 d S T P . .
O6 O 0.17586(13) 0.7864(4) 0.23411(9) 0.0160(4) Uani 1 1 d . . . . .
O7 O 0.11693(13) 0.8506(4) 0.35351(8) 0.0153(4) Uani 1 1 d . . . . .
O8 O 0.11542(14) 0.2591(4) 0.27178(9) 0.0192(4) Uani 1 1 d . . . . .
O9 O 0.18456(13) 0.2710(4) 0.41598(9) 0.0177(4) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ce1 O9 2.4622(18) . ?
Ce1 O9 2.4623(18) 2_565 ?
Ce1 O6 2.4920(18) 2_565 ?
Ce1 O6 2.4921(18) . ?
Ce1 O8 2.5068(19) . ?
Ce1 O8 2.5069(19) 2_565 ?
Ce1 O7 2.7537(19) 2_565 ?
Ce1 O7 2.7537(19) . ?
Ce1 Si2 3.3404(8) . ?
Ce1 Si2 3.3404(8) 2_565 ?
Ce1 Na2 3.9358(14) 7_565 ?
Ce1 Na2 3.9358(14) 8_655 ?
Sr1 O9 2.6425(18) 2_565 ?
Sr1 O9 2.6425(18) . ?
Sr1 O2 2.649(2) 2_565 ?
Sr1 O2 2.649(2) . ?
Sr1 O4 2.687(2) 2_565 ?
Sr1 O4 2.687(2) . ?
Sr1 O3 2.8242(19) 2_565 ?
Sr1 O3 2.8242(19) . ?
Sr1 Si1 3.4192(8) . ?
Sr1 Si1 3.4192(8) 2_565 ?
Sr1 Si1 3.6638(8) 2_575 ?
Sr1 Si1 3.6638(8) 1_545 ?
Zn1 O2 1.9610(19) 1_545 ?
Zn1 O2 1.9610(19) 2_565 ?
Zn1 O6 1.9849(18) 7_566 ?
Zn1 O6 1.9849(18) 8_646 ?
Zn1 Si2 2.9791(8) 8_646 ?
Zn1 Si2 2.9791(8) 7_566 ?
Na1 O4 2.307(2) . ?
Na1 O4 2.307(2) 5_566 ?
Na1 O1 2.397(2) 5_566 ?
Na1 O1 2.397(2) . ?
Na1 O3 2.5871(19) . ?
Na1 O3 2.5871(19) 5_566 ?
Na1 Si1 3.1032(8) 5_566 ?
Na1 Si1 3.1032(8) . ?
Na1 Si3 3.2884(7) . ?
Na1 Si3 3.2885(7) 5_566 ?
Na1 Si1 3.3707(8) 5_576 ?
Na1 Si1 3.3707(7) 1_545 ?
Na2 O8 2.412(2) 7_566 ?
Na2 O4 2.434(2) . ?
Na2 O2 2.472(2) . ?
Na2 O6 2.530(2) 7_566 ?
Na2 O5 2.653(2) 5_566 ?
Na2 O1 2.687(2) 5_566 ?
Na2 Si1 3.2170(13) . ?
Na2 Si2 3.2175(13) 7_566 ?
Na2 Si2 3.4700(13) 7_576 ?
Na2 Na2 3.642(3) 3_556 ?
Si1 O4 1.578(2) 1_565 ?
Si1 O2 1.602(2) . ?
Si1 O1 1.663(2) 5_566 ?
Si1 O3 1.6849(19) . ?
Si2 O8 1.583(2) 1_565 ?
Si2 O6 1.619(2) . ?
Si2 O5 1.6434(12) . ?
Si2 O7 1.6771(19) . ?
Si3 O9 1.586(2) . ?
Si3 O1 1.648(2) . ?
Si3 O7 1.6489(19) 1_545 ?
Si3 O3 1.6491(19) 1_545 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O9 Ce1 O9 76.77(9) . 2_565 ?
O9 Ce1 O6 113.78(7) . 2_565 ?
O9 Ce1 O6 130.62(7) 2_565 2_565 ?
O9 Ce1 O6 130.62(7) . . ?
O9 Ce1 O6 113.79(7) 2_565 . ?
O6 Ce1 O6 95.48(8) 2_565 . ?
O9 Ce1 O8 75.19(6) . . ?
O9 Ce1 O8 146.78(6) 2_565 . ?
O6 Ce1 O8 77.78(6) 2_565 . ?
O6 Ce1 O8 73.33(6) . . ?
O9 Ce1 O8 146.78(6) . 2_565 ?
O9 Ce1 O8 75.19(6) 2_565 2_565 ?
O6 Ce1 O8 73.34(6) 2_565 2_565 ?
O6 Ce1 O8 77.78(6) . 2_565 ?
O8 Ce1 O8 136.49(9) . 2_565 ?
O9 Ce1 O7 75.67(6) . 2_565 ?
O9 Ce1 O7 81.60(6) 2_565 2_565 ?
O6 Ce1 O7 57.66(6) 2_565 2_565 ?
O6 Ce1 O7 150.75(5) . 2_565 ?
O8 Ce1 O7 108.03(6) . 2_565 ?
O8 Ce1 O7 82.91(6) 2_565 2_565 ?
O9 Ce1 O7 81.60(6) . . ?
O9 Ce1 O7 75.67(6) 2_565 . ?
O6 Ce1 O7 150.75(5) 2_565 . ?
O6 Ce1 O7 57.67(6) . . ?
O8 Ce1 O7 82.91(6) . . ?
O8 Ce1 O7 108.03(6) 2_565 . ?
O7 Ce1 O7 150.92(7) 2_565 . ?
O9 Ce1 Si2 107.62(5) . . ?
O9 Ce1 Si2 96.13(5) 2_565 . ?
O6 Ce1 Si2 122.31(4) 2_565 . ?
O6 Ce1 Si2 27.65(4) . . ?
O8 Ce1 Si2 75.96(5) . . ?
O8 Ce1 Si2 92.80(5) 2_565 . ?
O7 Ce1 Si2 175.54(4) 2_565 . ?
O7 Ce1 Si2 30.02(4) . . ?
O9 Ce1 Si2 96.13(5) . 2_565 ?
O9 Ce1 Si2 107.62(5) 2_565 2_565 ?
O6 Ce1 Si2 27.64(4) 2_565 2_565 ?
O6 Ce1 Si2 122.31(4) . 2_565 ?
O8 Ce1 Si2 92.80(5) . 2_565 ?
O8 Ce1 Si2 75.96(5) 2_565 2_565 ?
O7 Ce1 Si2 30.02(4) 2_565 2_565 ?
O7 Ce1 Si2 175.54(4) . 2_565 ?
Si2 Ce1 Si2 149.72(3) . 2_565 ?
O9 Ce1 Na2 107.97(5) . 7_565 ?
O9 Ce1 Na2 147.74(5) 2_565 7_565 ?
O6 Ce1 Na2 77.86(5) 2_565 7_565 ?
O6 Ce1 Na2 38.75(5) . 7_565 ?
O8 Ce1 Na2 36.03(5) . 7_565 ?
O8 Ce1 Na2 105.24(5) 2_565 7_565 ?
O7 Ce1 Na2 130.67(4) 2_565 7_565 ?
O7 Ce1 Na2 73.62(4) . 7_565 ?
Si2 Ce1 Na2 51.70(2) . 7_565 ?
Si2 Ce1 Na2 103.60(2) 2_565 7_565 ?
O9 Ce1 Na2 147.74(5) . 8_655 ?
O9 Ce1 Na2 107.97(5) 2_565 8_655 ?
O6 Ce1 Na2 38.75(5) 2_565 8_655 ?
O6 Ce1 Na2 77.86(5) . 8_655 ?
O8 Ce1 Na2 105.24(5) . 8_655 ?
O8 Ce1 Na2 36.03(5) 2_565 8_655 ?
O7 Ce1 Na2 73.62(4) 2_565 8_655 ?
O7 Ce1 Na2 130.67(4) . 8_655 ?
Si2 Ce1 Na2 103.60(2) . 8_655 ?
Si2 Ce1 Na2 51.70(2) 2_565 8_655 ?
Na2 Ce1 Na2 85.18(4) 7_565 8_655 ?
O9 Sr1 O9 70.70(8) 2_565 . ?
O9 Sr1 O2 129.97(6) 2_565 2_565 ?
O9 Sr1 O2 114.33(6) . 2_565 ?
O9 Sr1 O2 114.33(6) 2_565 . ?
O9 Sr1 O2 129.97(6) . . ?
O2 Sr1 O2 99.46(8) 2_565 . ?
O9 Sr1 O4 76.59(6) 2_565 2_565 ?
O9 Sr1 O4 140.51(6) . 2_565 ?
O2 Sr1 O4 71.63(6) 2_565 2_565 ?
O2 Sr1 O4 83.52(6) . 2_565 ?
O9 Sr1 O4 140.52(6) 2_565 . ?
O9 Sr1 O4 76.59(6) . . ?
O2 Sr1 O4 83.53(6) 2_565 . ?
O2 Sr1 O4 71.63(6) . . ?
O4 Sr1 O4 141.34(8) 2_565 . ?
O9 Sr1 O3 81.07(6) 2_565 2_565 ?
O9 Sr1 O3 73.81(6) . 2_565 ?
O2 Sr1 O3 56.29(5) 2_565 2_565 ?
O2 Sr1 O3 154.02(5) . 2_565 ?
O4 Sr1 O3 79.90(6) 2_565 2_565 ?
O4 Sr1 O3 110.58(6) . 2_565 ?
O9 Sr1 O3 73.81(6) 2_565 . ?
O9 Sr1 O3 81.07(6) . . ?
O2 Sr1 O3 154.02(5) 2_565 . ?
O2 Sr1 O3 56.29(5) . . ?
O4 Sr1 O3 110.58(6) 2_565 . ?
O4 Sr1 O3 79.90(6) . . ?
O3 Sr1 O3 149.13(7) 2_565 . ?
O9 Sr1 Si1 96.23(5) 2_565 . ?
O9 Sr1 Si1 106.37(5) . . ?
O2 Sr1 Si1 125.58(4) 2_565 . ?
O2 Sr1 Si1 26.98(4) . . ?
O4 Sr1 Si1 98.47(5) 2_565 . ?
O4 Sr1 Si1 72.19(5) . . ?
O3 Sr1 Si1 177.09(4) 2_565 . ?
O3 Sr1 Si1 29.39(4) . . ?
O9 Sr1 Si1 106.37(5) 2_565 2_565 ?
O9 Sr1 Si1 96.23(5) . 2_565 ?
O2 Sr1 Si1 26.98(4) 2_565 2_565 ?
O2 Sr1 Si1 125.58(4) . 2_565 ?
O4 Sr1 Si1 72.19(5) 2_565 2_565 ?
O4 Sr1 Si1 98.48(5) . 2_565 ?
O3 Sr1 Si1 29.38(4) 2_565 2_565 ?
O3 Sr1 Si1 177.09(4) . 2_565 ?
Si1 Sr1 Si1 152.31(2) . 2_565 ?
O9 Sr1 Si1 67.55(4) 2_565 2_575 ?
O9 Sr1 Si1 138.25(4) . 2_575 ?
O2 Sr1 Si1 92.54(4) 2_565 2_575 ?
O2 Sr1 Si1 70.55(4) . 2_575 ?
O4 Sr1 Si1 22.78(5) 2_565 2_575 ?
O4 Sr1 Si1 140.73(4) . 2_575 ?
O3 Sr1 Si1 99.01(4) 2_565 2_575 ?
O3 Sr1 Si1 87.83(4) . 2_575 ?
Si1 Sr1 Si1 78.89(2) . 2_575 ?
Si1 Sr1 Si1 94.92(2) 2_565 2_575 ?
O9 Sr1 Si1 138.25(4) 2_565 1_545 ?
O9 Sr1 Si1 67.55(4) . 1_545 ?
O2 Sr1 Si1 70.55(4) 2_565 1_545 ?
O2 Sr1 Si1 92.54(4) . 1_545 ?
O4 Sr1 Si1 140.73(4) 2_565 1_545 ?
O4 Sr1 Si1 22.78(5) . 1_545 ?
O3 Sr1 Si1 87.83(4) 2_565 1_545 ?
O3 Sr1 Si1 99.01(4) . 1_545 ?
Si1 Sr1 Si1 94.92(2) . 1_545 ?
Si1 Sr1 Si1 78.90(2) 2_565 1_545 ?
Si1 Sr1 Si1 154.19(2) 2_575 1_545 ?
O2 Zn1 O2 104.34(11) 1_545 2_565 ?
O2 Zn1 O6 109.37(8) 1_545 7_566 ?
O2 Zn1 O6 115.66(8) 2_565 7_566 ?
O2 Zn1 O6 115.66(8) 1_545 8_646 ?
O2 Zn1 O6 109.37(8) 2_565 8_646 ?
O6 Zn1 O6 102.87(11) 7_566 8_646 ?
O2 Zn1 Si2 145.74(6) 1_545 8_646 ?
O2 Zn1 Si2 90.79(6) 2_565 8_646 ?
O6 Zn1 Si2 90.45(6) 7_566 8_646 ?
O6 Zn1 Si2 30.46(6) 8_646 8_646 ?
O2 Zn1 Si2 90.79(6) 1_545 7_566 ?
O2 Zn1 Si2 145.74(6) 2_565 7_566 ?
O6 Zn1 Si2 30.46(6) 7_566 7_566 ?
O6 Zn1 Si2 90.45(6) 8_646 7_566 ?
Si2 Zn1 Si2 93.52(3) 8_646 7_566 ?
O2 Zn1 Sr1 37.72(6) 1_545 1_545 ?
O2 Zn1 Sr1 82.96(6) 2_565 1_545 ?
O6 Zn1 Sr1 147.06(5) 7_566 1_545 ?
O6 Zn1 Sr1 95.14(5) 8_646 1_545 ?
Si2 Zn1 Sr1 117.508(14) 8_646 1_545 ?
Si2 Zn1 Sr1 123.966(15) 7_566 1_545 ?
O2 Zn1 Sr1 82.96(6) 1_545 . ?
O2 Zn1 Sr1 37.72(6) 2_565 . ?
O6 Zn1 Sr1 95.14(5) 7_566 . ?
O6 Zn1 Sr1 147.06(5) 8_646 . ?
Si2 Zn1 Sr1 123.966(15) 8_646 . ?
Si2 Zn1 Sr1 117.508(14) 7_566 . ?
Sr1 Zn1 Sr1 83.697(10) 1_545 . ?
O4 Na1 O4 180.0 . 5_566 ?
O4 Na1 O1 89.76(7) . 5_566 ?
O4 Na1 O1 90.24(7) 5_566 5_566 ?
O4 Na1 O1 90.24(7) . . ?
O4 Na1 O1 89.76(7) 5_566 . ?
O1 Na1 O1 180.0 5_566 . ?
O4 Na1 O3 92.51(6) . . ?
O4 Na1 O3 87.49(6) 5_566 . ?
O1 Na1 O3 63.15(6) 5_566 . ?
O1 Na1 O3 116.85(6) . . ?
O4 Na1 O3 87.49(6) . 5_566 ?
O4 Na1 O3 92.51(7) 5_566 5_566 ?
O1 Na1 O3 116.85(6) 5_566 5_566 ?
O1 Na1 O3 63.15(6) . 5_566 ?
O3 Na1 O3 180.0 . 5_566 ?
O4 Na1 Si1 96.65(5) . 5_566 ?
O4 Na1 Si1 83.35(5) 5_566 5_566 ?
O1 Na1 Si1 147.95(5) 5_566 5_566 ?
O1 Na1 Si1 32.05(5) . 5_566 ?
O3 Na1 Si1 147.12(4) . 5_566 ?
O3 Na1 Si1 32.88(4) 5_566 5_566 ?
O4 Na1 Si1 83.35(5) . . ?
O4 Na1 Si1 96.65(5) 5_566 . ?
O1 Na1 Si1 32.05(5) 5_566 . ?
O1 Na1 Si1 147.95(5) . . ?
O3 Na1 Si1 32.88(4) . . ?
O3 Na1 Si1 147.12(4) 5_566 . ?
Si1 Na1 Si1 180.0 5_566 . ?
O4 Na1 Si3 67.68(5) . . ?
O4 Na1 Si3 112.32(5) 5_566 . ?
O1 Na1 Si3 151.42(5) 5_566 . ?
O1 Na1 Si3 28.58(5) . . ?
O3 Na1 Si3 99.16(4) . . ?
O3 Na1 Si3 80.84(4) 5_566 . ?
Si1 Na1 Si3 56.43(2) 5_566 . ?
Si1 Na1 Si3 123.57(2) . . ?
O4 Na1 Si3 112.32(5) . 5_566 ?
O4 Na1 Si3 67.68(5) 5_566 5_566 ?
O1 Na1 Si3 28.58(5) 5_566 5_566 ?
O1 Na1 Si3 151.42(5) . 5_566 ?
O3 Na1 Si3 80.84(4) . 5_566 ?
O3 Na1 Si3 99.16(4) 5_566 5_566 ?
Si1 Na1 Si3 123.57(2) 5_566 5_566 ?
Si1 Na1 Si3 56.43(2) . 5_566 ?
Si3 Na1 Si3 180.0 . 5_566 ?
O4 Na1 Si1 155.89(5) . 5_576 ?
O4 Na1 Si1 24.11(5) 5_566 5_576 ?
O1 Na1 Si1 69.28(5) 5_566 5_576 ?
O1 Na1 Si1 110.72(5) . 5_576 ?
O3 Na1 Si1 67.81(4) . 5_576 ?
O3 Na1 Si1 112.19(4) 5_566 5_576 ?
Si1 Na1 Si1 107.44(2) 5_566 5_576 ?
Si1 Na1 Si1 72.56(2) . 5_576 ?
Si3 Na1 Si1 127.199(18) . 5_576 ?
Si3 Na1 Si1 52.800(18) 5_566 5_576 ?
O4 Na1 Si1 24.11(5) . 1_545 ?
O4 Na1 Si1 155.89(5) 5_566 1_545 ?
O1 Na1 Si1 110.72(5) 5_566 1_545 ?
O1 Na1 Si1 69.28(5) . 1_545 ?
O3 Na1 Si1 112.19(4) . 1_545 ?
O3 Na1 Si1 67.81(4) 5_566 1_545 ?
Si1 Na1 Si1 72.56(2) 5_566 1_545 ?
Si1 Na1 Si1 107.44(2) . 1_545 ?
Si3 Na1 Si1 52.801(18) . 1_545 ?
Si3 Na1 Si1 127.200(18) 5_566 1_545 ?
Si1 Na1 Si1 180.00(2) 5_576 1_545 ?
O8 Na2 O4 152.89(11) 7_566 . ?
O8 Na2 O2 84.94(8) 7_566 . ?
O4 Na2 O2 79.07(8) . . ?
O8 Na2 O6 74.27(7) 7_566 7_566 ?
O4 Na2 O6 88.78(8) . 7_566 ?
O2 Na2 O6 104.89(9) . 7_566 ?
O8 Na2 O5 89.84(7) 7_566 5_566 ?
O4 Na2 O5 100.13(7) . 5_566 ?
O2 Na2 O5 165.23(9) . 5_566 ?
O6 Na2 O5 60.35(5) 7_566 5_566 ?
O8 Na2 O1 110.07(8) 7_566 5_566 ?
O4 Na2 O1 80.64(7) . 5_566 ?
O2 Na2 O1 60.20(6) . 5_566 ?
O6 Na2 O1 163.02(9) 7_566 5_566 ?
O5 Na2 O1 134.46(8) 5_566 5_566 ?
O8 Na2 Si1 97.32(6) 7_566 . ?
O4 Na2 Si1 79.03(6) . . ?
O2 Na2 Si1 29.12(5) . . ?
O6 Na2 Si1 133.71(8) 7_566 . ?
O5 Na2 Si1 165.56(7) 5_566 . ?
O1 Na2 Si1 31.10(5) 5_566 . ?
O8 Na2 Si2 79.65(6) 7_566 7_566 ?
O4 Na2 Si2 96.19(6) . 7_566 ?
O2 Na2 Si2 134.60(8) . 7_566 ?
O6 Na2 Si2 29.77(5) 7_566 7_566 ?
O5 Na2 Si2 30.63(3) 5_566 7_566 ?
O1 Na2 Si2 164.29(8) 5_566 7_566 ?
Si1 Na2 Si2 163.45(7) . 7_566 ?
O8 Na2 Si2 23.48(5) 7_566 7_576 ?
O4 Na2 Si2 151.13(7) . 7_576 ?
O2 Na2 Si2 72.11(5) . 7_576 ?
O6 Na2 Si2 96.71(6) 7_566 7_576 ?
O5 Na2 Si2 107.23(5) 5_566 7_576 ?
O1 Na2 Si2 86.59(5) 5_566 7_576 ?
Si1 Na2 Si2 76.75(3) . 7_576 ?
Si2 Na2 Si2 102.59(3) 7_566 7_576 ?
O8 Na2 Na1 150.74(6) 7_566 . ?
O4 Na2 Na1 40.04(5) . . ?
O2 Na2 Na1 72.46(5) . . ?
O6 Na2 Na1 128.81(6) 7_566 . ?
O5 Na2 Na1 116.41(5) 5_566 . ?
O1 Na2 Na1 42.34(4) 5_566 . ?
Si1 Na2 Na1 54.25(2) . . ?
Si2 Na2 Na1 129.53(4) 7_566 . ?
Si2 Na2 Na1 127.82(3) 7_576 . ?
O8 Na2 Na2 57.84(6) 7_566 3_556 ?
O4 Na2 Na2 143.35(7) . 3_556 ?
O2 Na2 Na2 137.23(5) . 3_556 ?
O6 Na2 Na2 85.89(5) 7_566 3_556 ?
O5 Na2 Na2 46.65(5) 5_566 3_556 ?
O1 Na2 Na2 110.49(7) 5_566 3_556 ?
Si1 Na2 Na2 128.58(4) . 3_556 ?
Si2 Na2 Na2 63.43(3) 7_566 3_556 ?
Si2 Na2 Na2 65.50(2) 7_576 3_556 ?
Na1 Na2 Na2 131.61(7) . 3_556 ?
O8 Na2 Ce1 37.69(5) 7_566 7_566 ?
O4 Na2 Ce1 119.40(7) . 7_566 ?
O2 Na2 Ce1 88.31(6) . 7_566 ?
O6 Na2 Ce1 38.06(5) 7_566 7_566 ?
O5 Na2 Ce1 79.20(3) 5_566 7_566 ?
O1 Na2 Ce1 140.03(6) 5_566 7_566 ?
Si1 Na2 Ce1 113.95(4) . 7_566 ?
Si2 Na2 Ce1 54.56(2) 7_566 7_566 ?
Si2 Na2 Ce1 58.88(2) 7_576 7_566 ?
Na1 Na2 Ce1 153.31(5) . 7_566 ?
Na2 Na2 Ce1 75.03(4) 3_556 7_566 ?
O4 Si1 O2 118.61(11) 1_565 . ?
O4 Si1 O1 114.37(12) 1_565 5_566 ?
O2 Si1 O1 105.20(10) . 5_566 ?
O4 Si1 O3 110.52(10) 1_565 . ?
O2 Si1 O3 103.79(10) . . ?
O1 Si1 O3 102.69(10) 5_566 . ?
O4 Si1 Na1 144.05(8) 1_565 . ?
O2 Si1 Na1 97.33(8) . . ?
O1 Si1 Na1 49.88(7) 5_566 . ?
O3 Si1 Na1 56.47(7) . . ?
O4 Si1 Na2 135.53(8) 1_565 . ?
O2 Si1 Na2 48.67(8) . . ?
O1 Si1 Na2 56.57(8) 5_566 . ?
O3 Si1 Na2 113.93(8) . . ?
Na1 Si1 Na2 68.48(3) . . ?
O4 Si1 Na1 36.67(7) 1_565 1_565 ?
O2 Si1 Na1 155.12(8) . 1_565 ?
O1 Si1 Na1 92.83(8) 5_566 1_565 ?
O3 Si1 Na1 88.40(7) . 1_565 ?
Na1 Si1 Na1 107.44(2) . 1_565 ?
Na2 Si1 Na1 144.41(4) . 1_565 ?
O4 Si1 Sr1 136.05(9) 1_565 . ?
O2 Si1 Sr1 48.63(7) . . ?
O1 Si1 Sr1 109.49(8) 5_566 . ?
O3 Si1 Sr1 55.33(7) . . ?
Na1 Si1 Sr1 68.340(15) . . ?
Na2 Si1 Sr1 73.20(3) . . ?
Na1 Si1 Sr1 140.15(2) 1_565 . ?
O4 Si1 Sr1 41.26(8) 1_565 1_565 ?
O2 Si1 Sr1 96.30(8) . 1_565 ?
O1 Si1 Sr1 154.52(8) 5_566 1_565 ?
O3 Si1 Sr1 84.92(7) . 1_565 ?
Na1 Si1 Sr1 141.10(2) . 1_565 ?
Na2 Si1 Sr1 142.11(4) . 1_565 ?
Na1 Si1 Sr1 62.782(13) 1_565 1_565 ?
Sr1 Si1 Sr1 94.92(2) . 1_565 ?
O8 Si2 O6 116.64(11) 1_565 . ?
O8 Si2 O5 114.64(13) 1_565 . ?
O6 Si2 O5 106.13(10) . . ?
O8 Si2 O7 110.48(10) 1_565 . ?
O6 Si2 O7 100.83(10) . . ?
O5 Si2 O7 106.86(9) . . ?
O8 Si2 Zn1 79.16(8) 1_565 7_565 ?
O6 Si2 Zn1 38.43(7) . 7_565 ?
O5 Si2 Zn1 118.19(3) . 7_565 ?
O7 Si2 Zn1 124.55(8) . 7_565 ?
O8 Si2 Na2 138.74(8) 1_565 7_565 ?
O6 Si2 Na2 50.90(8) . 7_565 ?
O5 Si2 Na2 55.32(8) . 7_565 ?
O7 Si2 Na2 110.60(7) . 7_565 ?
Zn1 Si2 Na2 74.78(3) 7_565 7_565 ?
O8 Si2 Ce1 129.66(8) 1_565 . ?
O6 Si2 Ce1 45.59(7) . . ?
O5 Si2 Ce1 115.67(10) . . ?
O7 Si2 Ce1 55.24(7) . . ?
Zn1 Si2 Ce1 76.250(18) 7_565 . ?
Na2 Si2 Ce1 73.74(3) 7_565 . ?
O8 Si2 Na2 37.38(7) 1_565 7_575 ?
O6 Si2 Na2 104.52(8) . 7_575 ?
O5 Si2 Na2 87.06(9) . 7_575 ?
O7 Si2 Na2 146.30(8) . 7_575 ?
Zn1 Si2 Na2 69.35(3) 7_565 7_575 ?
Na2 Si2 Na2 102.59(3) 7_565 7_575 ?
Ce1 Si2 Na2 144.98(4) . 7_575 ?
O9 Si3 O1 110.80(11) . . ?
O9 Si3 O7 113.51(10) . 1_545 ?
O1 Si3 O7 105.83(10) . 1_545 ?
O9 Si3 O3 113.80(10) . 1_545 ?
O1 Si3 O3 105.70(10) . 1_545 ?
O7 Si3 O3 106.59(10) 1_545 1_545 ?
O9 Si3 Na1 79.48(8) . . ?
O1 Si3 Na1 44.09(7) . . ?
O7 Si3 Na1 149.02(8) 1_545 . ?
O3 Si3 Na1 91.86(7) 1_545 . ?
O9 Si3 Sr1 35.90(7) . . ?
O1 Si3 Sr1 105.81(8) . . ?
O7 Si3 Sr1 143.21(8) 1_545 . ?
O3 Si3 Sr1 82.23(7) 1_545 . ?
Na1 Si3 Sr1 62.405(12) . . ?
Si3 O1 Si1 132.13(14) . 5_566 ?
Si3 O1 Na1 107.33(9) . . ?
Si1 O1 Na1 98.07(9) 5_566 . ?
Si3 O1 Na2 127.33(10) . 5_566 ?
Si1 O1 Na2 92.33(9) 5_566 5_566 ?
Na1 O1 Na2 88.62(7) . 5_566 ?
Si1 O2 Zn1 119.13(12) . 1_565 ?
Si1 O2 Na2 102.22(10) . . ?
Zn1 O2 Na2 112.26(8) 1_565 . ?
Si1 O2 Sr1 104.39(9) . . ?
Zn1 O2 Sr1 115.36(9) 1_565 . ?
Na2 O2 Sr1 101.26(8) . . ?
Si3 O3 Si1 125.35(12) 1_565 . ?
Si3 O3 Na1 117.77(9) 1_565 . ?
Si1 O3 Na1 90.65(8) . . ?
Si3 O3 Sr1 130.12(10) 1_565 . ?
Si1 O3 Sr1 95.28(8) . . ?
Na1 O3 Sr1 85.36(6) . . ?
Si1 O4 Na1 119.22(11) 1_545 . ?
Si1 O4 Na2 123.47(11) 1_545 . ?
Na1 O4 Na2 97.21(8) . . ?
Si1 O4 Sr1 115.96(11) 1_545 . ?
Na1 O4 Sr1 94.38(7) . . ?
Na2 O4 Sr1 101.18(8) . . ?
Si2 O5 Si2 143.10(19) 3 . ?
Si2 O5 Na2 112.94(7) 3 7_565 ?
Si2 O5 Na2 94.05(7) . 7_565 ?
Si2 O5 Na2 94.05(7) 3 5_566 ?
Si2 O5 Na2 112.94(7) . 5_566 ?
Na2 O5 Na2 86.71(10) 7_565 5_566 ?
Si2 O6 Zn1 111.12(10) . 7_565 ?
Si2 O6 Ce1 106.76(9) . . ?
Zn1 O6 Ce1 121.39(9) 7_565 . ?
Si2 O6 Na2 99.34(10) . 7_565 ?
Zn1 O6 Na2 112.55(8) 7_565 7_565 ?
Ce1 O6 Na2 103.19(7) . 7_565 ?
Si3 O7 Si2 120.79(12) 1_565 . ?
Si3 O7 Ce1 130.31(10) 1_565 . ?
Si2 O7 Ce1 94.74(8) . . ?
Si2 O8 Na2 119.13(11) 1_545 7_565 ?
Si2 O8 Ce1 125.65(11) 1_545 . ?
Na2 O8 Ce1 106.28(8) 7_565 . ?
Si3 O9 Ce1 130.04(10) . . ?
Si3 O9 Sr1 123.49(9) . . ?
Ce1 O9 Sr1 106.26(7) . . ?
 
_refine_diff_density_max    1.271
_refine_diff_density_min   -0.643
_refine_diff_density_rms    0.160



